Journal of Physical Science and Application 7 (2) (2017) 18-26 doi: 10.17265/2159-5348/2017.02.003 D DAVID PUBLISHING

Low Cycle Fatigue, Creep-Fatigue and Relaxation-Fatigue Tests on P91

Carlo Cristalli, Pietro Agostini, Davide Bernardi, Nicola Bettocchi, Luigi Masotti and Sandro Storai ENEA CR Brasimone, Camugnano (BO) 40032, Italy

Abstract: Creep-fatigue is a damage mechanism where cyclic deformation damage (fatigue) is enhanced by creep damage and vice versa. Factors affecting the creep-fatigue damage are stress level (or, equivalently, strain range), temperature, hold time period, material softening/hardening and number of cycles. Moreover, environmental effects can accelerate the creep-fatigue interaction (oxidation, hot corrosion, irradiation, etc.). The activity described in this paper was planned to perform tests on 9Cr-1Mo ferritic/martensitic steel (P91) combining fatigue cycles and constant tensile and compressive holding periods. A preliminary basic fatigue characterization campaign in the LCF (low cycle fatigue) regime was carried out by performing a series of strain controlled tests, each at the same temperature (550 °C), using two different values for the total strain range (1% and 0.6%) and the same total strain rate (2×10-3 s-1). The tests were carried out with a strain ratio of –1, i.e., in fully reversed cyclic conditions. In this paper we illustrate the results obtained by testing in air P91 (9Cr-1Mo) ferritic/martensitic steel, introducing different dwell periods (either in strain or load control) and observing how these affect the fatigue life of the specimens. The final aim of the activity is to investigate how much detrimental is the effect of the holding periods on the fatigue life in order to validate the creep-fatigue interaction diagram presently adopted in RCC-MRx code for the P91 steel.

Key words: P91, creep-fatigue, fatigue damage, creep damage, interaction diagram, RCC-MRx, softening.

1. Introduction condition; Nf(fatigue)= Number of cycle to failure in LCF conditions; tH: hold time (hrs); tR: creep rupture Modified 9Cr-1Mo steel is a candidate steel for use time (hrs); D: failure criterion. The failure criterion in steam generators of nuclear power plants, to varies in agreement with the adopted standards. achieve a design life of 60 years and operational Criterion D is described by a curve in a “fatigue temperature 550 °C. To ensure the longevity and safe damage—creep damage” plot. A curve that bilinearly operation of a nuclear power plant, it is essential to connects (1, 0); (0.3, 0.3) and (0, 1) coordinates is prevent creep-fatigue damage and evaluate long-term employed in the RCC-MRx code [2] while the bilinear creep-fatigue life. The linear damage rule is the most correlation between (1, 0); (0.1, 0.01) and (0, 1) well-known method that is typically used to evaluate coordinates is adopted in the ASME code [3] (Fig. 1). creep-fatigue life. When the linear sum of fatigue One of the objectives of the present work is to clarify damage and creep damage of a material reaches a the discrepancy between the two curves of damage critical value, the material fails. Creep damage is limit. The first and second items in the left side of Eq. typically calculated using time fraction rule or (1) are fatigue damage and creep damage, respectively. ductility exhaustion approach. The following Eq. (1) The time fraction rule requires a creep rupture curve [1] is used to evaluate creep-fatigue life by the time to evaluate creep damage. In ASME III NH [3], JSME fraction rule: [4] and RCC-MRx [2] the calculation procedure of (1) creep damage utilizes the time-fraction approach, where, N = Number of cycle to failure in the tested while BS-R5 [5] is currently the only code following a

“ductility exhaustion” methodology. Corresponding author: Carlo Cristalli, research field: mechanical characterization of nuclear materials.

Low Cycle Fatigue, Creep-Fatigue and Relaxation-Fatigue Tests on P91 19

Fig. 1 Creep fatigue Interaction Diagram according to RCC-MRx and ASME.

Concerning the assessment of the creep-fatigue the holding periods on the fatigue life in order to interaction damage, several researchers have validate the creep-fatigue interaction diagram adopted previously proposed different approaches based on in RCC-MRx code for the P91 steel. hysteresis energy [6-9]. Takahashi et al. [9] evaluated 2. Material and Experimental Procedures creep damage on the basis of inelastic strain-energy density rate and creep-fatigue life using the linear sum The experimental set-up used to performr LCF (low of fatigue damage and creep damage. Other works cycle fatigue), CF (creep fatigue) and RF (relaxation propose innovative methods to evaluate creep-fatigue fatigue) tests consists of the following components: life on the basis of fracture energy [10-12] considering hydraulic press (100 kN), load cell (operation range: ± as time dependent the change in fracture energy. 100 kN), extensometer (12 mm gauged length) and Kimura et al. [13] have proposed a method for induction furnace (6 kW). An extensive optimization predicting creep life called the “region splitting process has been carried out on the induction furnace analysis method”. In this method, creep rupture data shape in order to keep the temperature profile constant are divided into high-stress and low-stress regions along the gauged length, achieving a tolerance within with a boundary condition of one half of the 0.2% ±2 °C. A Control Unit with embedded software allows offset yield stress. The region splitting analysis great flexibility in mixing fatigue cycling with creep method for creep rupture curves has been taken into hold times. account in the 2012 JSME code. The samples for the tests were manufactured The activity reported in this paper was planned to according to ASTM 2714-099 [14] and have undergone perform tests on 9Cr-1Mo ferritic/martensitic steel statistic quality controls after production in order to (P91) at 550 °C combining fatigue cycles and constant verify their fulfilment to specifications in terms of tensile holding periods (in both creep-fatigue and surface roughness and dimensional tolerances. The relaxation-fatigue mode). The final aim of the activity specimens have been obtained from the 12 mm thick is to investigate how much detrimental is the effect of 9Cr1MoVNb plate manufactured by Industeel. The

20 Low Cycle Fatigue, Creep-Fatigue and Relaxation-Fatigue Tests on P91 chemical composition of the material is reported in during the hold-time. The load, on the other hand, is Table 1. The plate has undergone the following the feedback signal in tensile and compressive peaks thermal treatments: austenitization (1,060 °C—4 h), and becomes the controlled parameter during the water quenching, tempering (760 °C—3 h 20 min) and hold-time (Fig. 2). air cooling. Different from CF tests, in RF tests, the strain CF (creep fatigue) and RF (relaxation fatigue) tests remains the controlled parameter for the whole differ from standard LCF tests by the interposition of duration of the cycle, both in tensile and compressive hold-times within the cyclic testing. During CF tests, peaks and during the hold-time. The load, on the other the stress level is held constant during holding periods. hand, remains the feedback signal both in tensile and The strain is the controlled parameter in tensile and compressive peaks and during the hold-time (Fig. 3). compressive peaks and it becomes the feedback signal In all of the cases, the fatigue strain was controlled

Table 1 Nominal chemical composition of P91 steel supplied by Industeel (wt%). C Si Mn P Cr Mo Ni Al Cu Nb Ti V N Fe 0.102 0.22 0.38 0.021 8.99 0.89 0.11 0.015 0.06 0.06 0.003 0.21 0.044 Bal.

Fig. 2 CF cycle; HT tension 12 s; stress-strain behaviour.

Fig. 3 RF cycle; HT tension 600 s; stress-strain behaviour at the beginning (left), and end of HT (right).

Low Cycle Fatigue, Creep-Fatigue and Relaxation-Fatigue Tests on P91 21

in terms of total strain (elastic + plastic), which was Besides the LCF (low cycle fatigue), the CF (creep measured and controlled by the extensometer. The fatigue) and the RF (relaxation fatigue) tests, a series wave shape was triangular and the parameters of the of creep rupture tests has been performed, in test (total strain range, strain rate and frequency) are agreement with ASTM E139-11 standards [15]. The listed below: tests have been carried out using single lever MAYES

tot =1%, 0.6% machines with auto-levelling arm device. A three

zones P.I.D. controlled furnace and the utilization of S 210 type thermocouples allow the temperature gradient to Frequency 0.1 Hz be maintained at ± 1 °C along the gauge length. In the following figures the evolution of the 3. Experimental Outcomes and Analysis of hysteresis cycles is reported, both for CF tests (Fig. 4) Results and for RF tests (Fig. 5). The flattening of the hysteresis cycles in the end of life with respect to the A preliminary basic fatigue characterization beginning is noticeable. This is due to cyclic softening campaign in the LCF regime was carried out. which is characteristic of ferritic/martensitic steels. Two values of fatigue strain have been considered in the

Fig. 4 CF hysteresis cycles;= 1%; HT tension 12 s.

Fig. 5 RF hysteresis cycles; = 1%; HT tension 600 s.

22 Low Cycle Fatigue, Creep-Fatigue and Relaxation-Fatigue Tests on P91

experiments: 0.6% and 1%. The resulting trends of the criterion to estimate the cycles to fracture was that of stabilized load are reported in the next graph (Fig. 6). 25% load drop, according to ASTM 2714-09 [14]. Then, for each strain range, several HT (hold time) The pictures of the fractured section of the specimen durations have been chosen based on literature sources used in the CF test (600 s HT) are reported in Fig. 7. [16-18], both in CF and in RF condition. The stress The appearance of the fracture surface reveals a mixed controlled creep-fatigue hold times are expected to be ductile-fatigue fracture mode. more detrimental than the strain controlled The test conditions and the corresponding results relaxation-fatigue hold times. Thus, concerning the are summarized in Table 2 in terms of cycles to creep-fatigue hold times, the short durations (12 s and fracture, corresponding fatigue damage and creep 120 s) are addressed in the tests performed with 1% damage. Details of the calculations are reported in the fatigue strain range while the long durations (600 s following paragraphs. The complete experimental data and 1,800 s) are used in the tests with 0.6% fatigue of each performed test were made available on the strain range. These durations of the hold times have on-line Mat-DB database, managed by JRC [19]. been chosen in order to balance the detrimental effects The results of the performed creep rupture tests, in of creep and fatigue for each considered value of the terms of time to rupture, are reported in the graph strain range; furthermore the choice was made in below (Fig. 8). The achieved experimental points are agreement with previous published works dealing compared to the minimum and average values for P91, with creep-fatigue tests on P91 [16-18]. The adopted according to RCC-MRx [2]. The experimental points

Fig. 6 Trends of the stabilized load for LCF tests (0.6% and 1% strain range).

Fig. 7 Fracture of the specimen tested with CF HT 600 s; = 0.6%.

Low Cycle Fatigue, Creep-Fatigue and Relaxation-Fatigue Tests on P91 23

Table 2 Test matrix with number of cycles to fracture and relative damage achieved in each experimental condition. Hold Time Δє Testing Hold Time duration Number of cycles Fatigue Creep Test # tot Type duration in temperature (°C) in tension (min) to failure N damage damage [%] compression(min) f 1 0.6 LCF 550 - - 4,550 0.96 0 1 0.6 LCF 550 - - 4,222 0.84 0 2 1 LCF 550 - - 1,379 0.88 0 2 1 LCF 550 - - 1,590 1.02 0 3 0.6 CF 550 10 - 1,620 0.34 2.47 3 0.6 CF 550 10 - 1,470 0.31 2.33 4 0.6 CF 550 30 - 783 0.16 3.52 4 0.6 CF 550 30 - 775 0.16 2.89 5 1 CF 550 2 - 902 0.58 1.45 5 1 CF 550 2 - 882 0.57 1.16 6 1 CF 550 0,2 - 1,145 0.73 0.63 6 1 CF 550 0,2 - 1,010 0.65 0.81 7 0.6 RF 550 10 - 4,750 1 0.45 8 0.6 RF 550 10 10 2,534 0.53 0.45* 9 1 RF 550 10 - 1,503 0.96 1.07 9 1 RF 550 10 - 1,805 1.16 1.07 10 1 RF 550 30 - 1,934 1.24 0.52 11 1 RF 550 10 10 1,270 0.82 0.57* * The creep damage has not been calculated for the hold times in compression.

Fig. 8 Times to rupture for the performed creep rupture tests; comparison with RCC-MRx values (average and minimum duration).

24 Low Cycle Fatigue, Creep-Fatigue and Relaxation-Fatigue Tests on P91

Fig. 9 Creep-fatigue interaction diagram on a double-logarithmic scale with plotted experimental points.

appear to be located in the range between the Ti = Time to rupture corresponding to the load level minimum and the average RCC-MRx values. recorded at each hold time of the test. A fourth degree polynomial function has been used to interpolate the 3.1 The Fatigue Damage RCC- MRx [2] time to rupture experimental values.

The fatigue damage has been evaluated through the Nf = Number of cycles to obtain 25% of load following formulation: decrease in each test, according to ASTM E2714-09

[14]. (2) 3.3 The Interaction Diagram where, Nf = Number of cycles to obtain 25% of load decrease in each test, according to ASTM E2714-09 As we can observe in Fig. 9, CF and RF [14]; experimental points fall in the “unsafe” zone of the

Nmax = Maximum number of allowable strain cycles, creep-fatigue interaction diagram, as expected. The as determined on the best fit experimental fatigue interaction curve is plotted according to RCC-MRx [2] curve deduced by the RCC-MRx design fatigue curve and ASME [3] on a double-logarithmic scale diagram. at 550 °C multiplied by a factor of 2 in the strain 4. Conclusions range or a factor of 20 in the number of cycles whatever is the most conservative condition. Several combinations of hold time durations in different conditions (CF and RF type) have been 3.2 The Creep Damage experimented; the CF hold times lead to a higher The creep damage has been evaluated through the creep damage and a shorter fatigue life than the following formulation: corresponding RF hold times, as expected. The fatigue

life appears deeply affected, in terms of reduction in ∑ (3) the number of cycles to failure, by the presence of where, Tht = Duration of the hold time period in each tensile CF hold times, while no marked life reduction considered kind of test, ranging from 12 s to 1,800 s; can be noticed due to the RF tensile hold times; this

Low Cycle Fatigue, Creep-Fatigue and Relaxation-Fatigue Tests on P91 25 test condition appears even beneficial for some of the [13] Kimura, K., Sawada, K., and Kushima, H. 2010. Vessels Pip. Div. Conf. PVP2010-25297. ASME Press. tested specimens. The most critical tests, namely the [14] ASTM E2714-09—Standard Test Method for closest points to the RCC-MRx curve, are the “RF Creep-Fatigue Testing. mixed”, namely the ones with same HT duration [15] ASTM E139-11—Standard Test Methods for conducting repeated both in tension and compression. This Creep, Creep-rupture and Stress-Rupture Tests。 depends on the fact that creep damage has not been [16] Fournier, B. et al. 2011. “Comparison of Variuos 9-12Cr Steels under Fatigue and Creep-Fatigue Loadings at High calculated for compressive hold times. The main Temperature.” Materials Science and Engineering A 528: outcome of this activity concerns the update of the 6034-945. RCC-MRx Code, as long as this experimental [17] Fournier, B. et al. 2009. “Creep-Fatigue Interactions in a campaign resulted successful in validating the 9 Pct Cr-1 Pct Mo Martensitic Steel: Part I. Mechanical Test Results.” Metallurgical and Materials Transactions creep-fatigue interaction diagram. Every experimental A 40A: 321-9. condition, in fact, falls in the “unsafe” zone of the [18] Fournier, B. et al. 2008. “Creep-Fatigue-Oxidation creep-fatigue interaction diagram, according to the Interactions in a 9Cr–1Mo Martensitic Steel. Part I: RCC-MRx curve. Effect of Tensile Holding Period on Fatigue Lifetime.” International Journal of Fatigue 30: 649-62. Acknowledgements [19] https://odin.jrc.ec.europa.eu. [20] Kawasaki, N. et al. 1999. Trans. 15th Int. Conf. Struct. This work was carried out in the frame of the EU Mech. Reactor Technol. IV: 161. Project MATTER (WP7-Task 7.1-Grant Agreement [21] Asayama, T., and Tachibana, Y. 2007. “Collect Available Creep-Fatigue Data and Study Existing Creep-Fatigue no. 269706). Evaluation Procedures for Grade 91 and Hastelloy XR, DOE/ASME Generation IV Materials Project, a report on References Task 5 submitted to ASME ST-LLC, Revision 3 Final [1] Nagae, Y. 2013. Materials Science & Engineering A 560: Report.” JAEA. 752-8. [22] Filacchioni, G. 2006. Effects of Hold-Times and Other [2] AFCEN RCC-MRx Code. 2012. Design and Construction Testing Parameters on Fatigue Behaviour of Eurofer 97 Rules for Mechanical Components of Nuclear Base Metal. Final Report for task TW2-TTMS-002 of the Installations. EFDA Technology Programme. [3] ASME boiler and pressure vessel code. 2007. Section III [23] Pohja, R., Holmström, S., Nilsson, K.-F., Payten, W., Lee, Div. 1 Sub-Section NH. New York, USA: ASME. H.-Y., and Aktaa, J. 2014. “Creep-Fatigue Interaction [4] Onizawa, T., Nagae, Y., Wakai, T., and Asayama, T. Rules for P91.” MATTER—Deliverable D4.5, 2009. ASME Pressure Vessels Pip. Div. Conf. PVP2009 EURATOM FP7 Grant Agreement no. 269706. 77984. [24] Holmstrom, S., Pohaj, R., and Payten, W. 2014. [5] R5. 2003. Assessment Procedure for the High Temperature “Creep-Fatigue Interaction Models for Grade 91 Steel. Response of Structures. Gloucester, UK: British Energy. ASTM, Materials Performance and Characterization.” [6] Ostergren, W. J. 1976. J. Test. Eval. 4: 327-39. DOI: 10.1520/MPC20130054, Published Online. [7] Leis, B. N. 1977. J. Pressure Vessel Technol.: 524-33. [25] Pohja, R., Holmström, S., and Lee, H.-Y. 2014. [8] Payten, W. M., Dean, D. W., and Snowden, K. U. 2009. “Recommendation for Creep and Creep-Fatigue Vessels Pip. Div. Conf. PVP2009-77208. ASME Press. Assessment for P91.” MATTER—Deliverable D4.6, [9] Takahashi, Y., Dogan, B., and Gandy, D. 2009. Vessels EURATOM FP7 Grant Agreement no. 269706. Pip. Div. Conf. PVP2009-77990. ASME Press. [26] EPRI Techincal Report. 2013. Final Report on [10] Masanori, A., Nobuhiro, I., Kikuchi, K., and Yasuhiro, E. Round-Robin Conducted in Support of Standard Test 2012. “Effect of Ratchet Strain on Fatigue and Method for Creep-Fatigue Testing, nr. 3002001719, Creep-Fatigue Strength of Mod.9Cr-1Mo Steel.” Nuclear Electric Power Research Institute. Engineering and Design 247: 66-75. [27] Holmström, S., and Auerkari, P. 2006. “Robust [11] Nagae, Y., Takaya, S., and Asayama, T. 2009. J. Solid Prediction of Full Creep Curves from Minimal Data and Mech. Mater. Eng. 3: 449-56. Time to Rupture Model.”Energy Materials, Materials [12] Nagae, Y., and Takaya, S. 2011. J. Soc. Mater. Sci. Jpn60 Science & Engineering for Energy Systems1: 249-55. (2): 108-15. [28] Holmström, S. 2010. “Engineering Tools for Robust

26 Low Cycle Fatigue, Creep-Fatigue and Relaxation-Fatigue Tests on P91

Creep Modeling.” Dissertation, VTT Publications 728, [31] Tai, A. 2009. “Update and Improve Subsection NH VTT, Espoo, ISBN 978-951-38-7378-3. Alternative Simplified Creep-Fatigue Design Methods.” [29] Wilshire, B., Scharming, P. J., and Hurst, R. 2009. “A [32] Manson, S. S. 1968. “A Simple Procedure for Estimating New Approach to Creep Data Assessment.” Material High-Temperature Low Cycle Fatigue.” Experimental Science and Engineering A 510-511: 3-6. Mechanics 8 (8): 349-55. [30] NIMS Atlas of Creep Deformation Property No. D-1, [33] Holmström, S., and Auerkari, P. 2013. “A Robust Model Creep deformation properties of 9Cr-1Mo-V-Nb steel for Creep-Fatigue Life Assessment.” Mater. Sci. Eng. A tubes for boiler and heat exchangers, 2007. 559: 333-5.